- Home
- Documents
*5 Optical Fibers 116 Chapter 5 Optical Fibers wavelength. The basic material used in the manufacture*

prev

next

out of 34

View

0Download

0

Embed Size (px)

111

5 Optical Fibers Takis Hadjifotiou

Telecommunications Consultant

Introduction

Optical fi ber communications have come a long way since Kao and Hockman (then at the Standard Telecommunications Laboratories in England) published their pioneering paper on communication over a piece of fi ber using light (Kao & Hockman, 1966). It took Robert Maurer, Donald Keck, and Peter Schultz (then at Corning Glass Works–USA) four years to reach the loss of 20 dB/km that Kao and Hockman had considered as the target for loss, and the rest, as they say, is history. For those interested in the evolution of optical communica- tions, Hecht (1999) will provide a clear picture of the fi ber revolution and its ramifi cations.

The purpose of this chapter is to provide an outline of the performance of fi bers that are fabricated today and that provide the pathway for the transmission of light for communications.

The research literature on optical fi bers is vast, and by virtue of necessity the references at the end of this chapter are limited to a few books that cover the topics outlined here.

The Structure and Physics of an Optical Fiber

The optical fi bers used in communications have a very simple structure. They consist of two sections: the glass core and the cladding layer (Figure 5.1).

The core is a cylindrical structure, and the cladding is a cylinder without a core. Core and cladding have different refractive indices, with the core having a refractive index, n1, which is slightly higher than that of the cladding, n2. It is this difference in refractive indices that enables the fi ber to guide the light. Because of this guiding property, the fi ber is also referred to as an “optical waveguide.” As a minimum there is also a further layer known as the secondary cladding that does not participate in the propagation but gives the fi ber a minimum level of protection. This second layer is referred to as a coating.

112 Chapter 5 Optical Fibers

The basics of light propagation can be discussed with the use of geometric optics. The basic law of light guidance is Snell’s law (Figure 5.2a). Consider two dielectric media with different refractive indices and with n1 > n2 and that are in perfect contact, as shown in Figure 5.1. At the interface between the two dielectrics, the incident and refracted rays satisfy Snell’s law of refraction—that is,

n n1 1 2 2sin sinφ φ= (5.1)

or

sin sin

φ φ

1

2

2

1 = n

n (5.2)

In addition to the refracted ray there is a small amount of refl ected light in the medium with refractive index n1. Because n1 > n2 then always f2 > f1. As the angle of the incident ray increases there is an angle at which the refracted ray emerges parallel to the interface between the two dielectrics (Figure 5.2(b)).

This angle is referred to as the critical angle, fcrit, and from Snell’s law is given by

sinφcrit = n n

2

1 (5.3)

Core

Cladding

(a) (b)

n1 > n2

n2

Secondary Cladding

Secondary Cladding

Cladding

Core

Fig. 5.1 (a) Cross section and (b) longitudinal cross section of a typical optical fi ber.

f1 fcrit

f2

n1

n2

Incident Ray

Transmitted Ray

Partially Reflected Ray

f tr = 90°

n1

n2

Incident Ray

Transmitted Ray

n1 > n2

(a) (b)

Fig. 5.2 Snell’s law.

If the angle of the incident ray is greater than the critical angle, the ray is refl ected back into the medium with refractive index n1. This basic idea can be used to propagate a light ray in a structure with n1 > n2, and Figure 5.3 illustrates this idea.

The light ray incident at an angle greater than the critical angle can propagate down the waveguide through a series of total refl ections at the interface between the two dielec- trics. The ray shown in Figure 5.3 is referred to as a “meridional ray” because it passes through the axis of the fi ber. For rays not satisfying this condition, see Senior (1992). Clearly, the picture of total internal refl ection assumes an ideal situation without imperfections, discontinuities, or losses. In a real-world fi ber, imperfections will introduce light that is refracted as well as refl ected at the boundary. In arriving at the basic idea of light propaga- tion, it was assumed that somehow the ray has been launched into the fi ber.

For a ray to be launched into the fi ber and propagated it must arrive at the interface between the two media (with different refractive indices) at an angle that is at minimum equal to fcrit and in general less than that. Figure 5.4 illustrates the geometry for the deriva- tion of the acceptance angle. To satisfy the condition for total internal refl ection, the ray arriving at the interface, between the fi ber and outside medium, say air, must have an angle of incidence less than qacc, otherwise the internal angle will not satisfy the condition for total refl ection, and the energy of the ray will be lost in the cladding.

Consider that a ray with an incident angle less than the qacc, say q1, enters the fi ber at the interface of the core (n1) and the outside medium, say air (n0), and the ray lies in the meridional plane. From Snell’s law at the interface we obtain

n n0 1 1 2sin sinθ θ= (5.4)

n1

n2

n2

Geometric Axis of the Structure

n1n2

Refractive Index

Fig. 5.3 Light guidance using Snell’s law.

q1

Fiber Core

n1

n2Cladding

n0 Cladding n2

q j j

2A

B

C Acceptance Cone

Fig. 5.4 Geometry for the derivation of the acceptance angle.

The Structure and Physics of an Optical Fiber 113

114 Chapter 5 Optical Fibers

From the right triangle ABC (Figure 5.4), the angle f is given by

φ π θ= − 2 2

(5.5)

where the angle f is greater than the critical angle. Substituting equation 5.5 into equation 5.4 we obtain

n n0 1 1sin cosθ φ= (5.6)

In the limit as the incident angle, q1, approaches qacc, the internal angle approaches the critical angle for total refl ection, fcrit. Then, by introducing the trigonometric relation sin2f + cos2f = 1 into equation 5.4, we obtain

n n n n n n

n n0 1 1 1 2 1 2 1 2

1

2 1 2

1 2

21 1sin cos ( sin ) (θ φ φ= = − = − ( )⎛⎝⎜ ⎞⎠⎟ = −/ /

22 1 2) / (5.7)

This equation defi nes the angle within which the fi ber can accept and propagate light and is referred to as the “Numerical Aperture” (NA).

NA acc /= = −n n n0 12 22 1 2sin ( )θ (5.8)

When the medium with refractive index n0 is air, the equation for the NA of the glass fi ber simplifi es to

NA acc /= = −sin ( )θ n n12 22 1 2 (5.9)

This equation states that for all angles of incident where the inequality 0 ≤ q1 ≤ qacc is satisfi ed the incident ray will propagate within the fi ber. The parameter NA expresses the propensity of the fi ber to accept and propagate light within the solid cone defi ned by an angle, 2qacc. The equation for the NA can be also expressed in terms of the difference between the refractive indices of core and cladding—that is,

Δ = − ≈ −n n n

n n n

1 2

2 2

1 2

1 2

12 (5.10)

With these simplifi cations the NA can now be written as

NA /= n1 1 22( )Δ (5.11)

To appreciate the numbers involved, consider a fi ber made of silica glass whose core refractive index is 1.5 and that of the cladding is 1.46. The fcrit and the NA of the fi ber are calculated to be

φcrit = ( ) = ( ) = °− −sin sin .. .1 21 1 1 46 1 50

76 73n n

NA / / /= − = − = − =( ) ( . . ) ( . . ) .n n12 22 1 2 2 2 1 2 1 21 50 1 46 2 25 2 13 0 346

θacc NA= = = °− −sin sin . .1 1 0 346 20 24

If one uses the equation for the approximation of NA, equation 5.11, the result is

NA / /

/≈ = × × −( )( ) = × × =n1 1 2 1 2 1 22 1 5 2 1 50 1 461 5 1 5 2 0 0266 0( ) . . .. . ( . )Δ ..346

If the ray does not lie in the meridional plane, the analysis for obtaining the NA is slightly more complex.

The discussion up to now has been based on the launching and propagation of a single ray. Because all the rays with a refl ection angle less that the critical angle can propagate, it is expected that a number of rays will propagate provided they can be launched into the fi ber. The class of fi ber that can support the simultaneous propagation of a number of rays is known as multimode fi ber. The term “mode” is used in a more sophisticated analysis of light propagation using Maxwell’s equations, and it corresponds to one solution of the equations. Therefore, the concept of a ray and a mode are equivalent, and in the rest of this chapter the term “mode” will be used.

A fi ber that allows the propagation of one mode only is called a single-mode fi ber. A fi ber can be multimode or single mode, and the behavior depends on the relative dimensions of the core and the wavelength of the propagating light. Fibers with a core diameter much larger than the wavelength of the launched light will support many propagating modes, and the propagating conditions can be analyzed with geometric optics. A fi ber with a core diameter similar to that of the light wavelength supports only one propagation mode. Figure 5.5 illustrates these